Laboratory 4 Bending Test of Materials

Save this PDF as:

Size: px
Start display at page:

Transcription

1 Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective Bend or flexure testing is common in springs and brittle materials whose failure behaviours are linear such as concretes, stones, woods, plastics, glasses and ceramics. Other types of brittle materials such as powder metallurgy processed metals and materials are normally tested under a transverse flexure. Bend test is therefore suitable for evaluating strength of brittle materials where conduction of tensile test and interpretation of test result of material is difficult and sometimes impossible. After completion of this experiment, students should be able to. conduct 3-point bend test and investigate responses of materials when subjected to bending.2 determine flexural bend strength and elastic modulus of brittle material, and.3 analyse statistical nature of the test data and determine the Weibull modulus of the brittle materials 2. Materials and Equipment 2. Bend samples 2.2 Universal testing machine 2.3 Vernia calliper 3. Experimental Procedure 3. Bend test of materials 3.. Measure the width and thickness of the specimen. Mark on the locations where the load will be applied under three-point bending Place the sample carefully on to the stage of 3-point bending fixture of a universal testing machine. Make sure that the loading point is placed on to the marked location Carry out the bend test until failure takes place Construct the load-extension or load-deflection curve to calculate the flexural bend strength and elastic modulus of the specimen Repeat steps 3.. to 3..4 to conduct bend tests of other specimens. 3.7 Complete the Data Sheet, Table Statistical analysis of data 3.2. Conduct 3-point bend test of at least 5 glass specimens following steps 3.. to Note the breaking loads and then determine flexural bend strength (MOR) of these specimens.

2 3.2.3 Arrange them in descending order, rank them and determine their failure probability, P f Construct ln ( ln ( P f )) vs. ln (MOR) curve and determine Weibull constants m and Results 4. Display the test data in the Table. 4.2 Determine bend strength, elastic modulus and flexural strength (MOR) of the material. 4.3 Determine Weibul modulus of the material and comment on the degree of homogeneity of the material. 5. Discussion 5. Answer the following questions: (a) Give three examples of engineering applications that involve bending properties of materials. (b) What would you expect if the bending experiment has been carried out at elevated temperature? (c) Why does the presence of cracks in ductile materials present not much problem when compare with brittle material? (d) Explain why flexural strength of brittle material is always higher than tensile strength of the respective material. (e) (f) Determine the flexural strength of material testing using 4-point bend test. What conclusion can you draw from the Weibull modulus value of a test sample? (g) Compare and explain the Weibull modulus of cast and wrought aluminium alloys. 2

3 Table 3.: Data Sheet for Bend Test Sample identification Symbol Unit Value 2 3 Average Material Width of sample w mm Thickness of sample t mm Span length of sample L mm Fracture load P f kn Flexural Bend Strength (MOR) fb MPa Elastic Modulus E b GPa **Provide all calculations in separate pages. Signature with Date of the Instructor/Course Tutor 3

4 6.0 Theoretical Background 6. Introduction Preparing specimens from brittle materials, such as ceramics and glasses, for direct tension tests is difficult because of the problems involved in shaping and machining them to proper dimensions. Furthermore, such specimens are sensitive to surface defects and notches, and clamping brittle test specimens for testing is difficult. Also, improper alignment of the test specimen may result in a non-uniform stress distribution along the cross section and ultimate premature failure. A commonly used test method for measuring strength of brittle materials such as ceramics and glasses is the bend or flexure test. The test specimen can have a circular, square, or rectangular cross section and is uniform along the complete length. Such a specimen is much less expensive to fabricate than a tensile specimen. The test is conducted with the same kind of universal testing machine used for tensile and compressive strength measurements. The test specimen is supported at the ends and the load is applied either at the centre (threepoint loading) or at two positions (four-point loading), Fig. 6.. The longitudinal stresses in the specimens are tensile at their lower surfaces and compressive at their upper surfaces. The bend or flexural strength is defined as the maximum uniaxial tensile strength at failure and it is often referred to as the flexural strength or modulus of rupture (MOR). P P/2 P/2 L/2 P/2 L P/2 c = t/2 a P/2 L P/2 c = t/2 (a) Figure 6.: Two bend-test methods for brittle materials: (a) three-point bending; (b) four-point bending. The areas on the beams represent the bending moment diagrams. Note the region of constant maximum bending moment in (b); by contrast, the maximum bending moment occurs only at the centre of the specimen in (a). (b) Three-point testing is still an option, but four-point is preferred since more material is exposed to high stress. Also, because of the larger volume of material subjected to the same bending moment in Fig. 6.b, there is a higher probability that defects exist in this volume than in that in Fig. 6.a. Consequently, the four-point test gives a lower modulus of rupture than the three-point test. Figure 6.2 illustrates three-point bending arrangement which is capable of 80 bend angle for welded materials. 6.2 Three-Point Bend Test of Brittle Materials Considering a three point bend test of an elastic material, when the load P is applied at the mid-span of specimen in an x-y plane, stress distribution across the specimen thickness (t) is demonstrated in Fig The stress is essentially zero at the neutral axis N-N. Stresses in the y axis in the positive direction represent tensile stresses whereas stresses in the negative direction represent compressive stresses. Within the elastic range, brittle materials show a linear relationship of load and deflection where yielding occurs on a thin layer of the 4

5 Figure 6.2: Example of a weld plate bend tested under a three-point bend arrangement. specimen surface at the mid-span, Fig. 6.3a. This in turn leads to crack initiation which finally proceeds to specimen failure. Ductile materials however provide load-deflection curves which deviate from a linear relationship before failure takes place as opposed to those of brittle materials previously mentioned. Furthermore, it is also difficult to determine the beginning of yielding in this case. The stress distribution of a ductile material after yielding is given in Fig. 6.3b. Therefore, it can be seen that bend testing is not suitable for ductile materials due to difficulties in determining the yield point of the materials under bending and the obtained stress-strain curve in the elastic region may not be linear. The results obtained might not be validated. As a result, the bend test is therefore more appropriate for testing brittle materials whose stress-strain curves (Fig. 6.4) show its linear elastic behaviour just before the materials fail. P w x P/2 z y P/2 c c t/2 t/2 t/2 t/2 c c (a) Figure 6.3: Stress distributions in a rectangular bar when (a) elastically bended and (b) after yielding (b) 5

6 Figure 6.4: Flexural stress and flexural strain relationship Determination of flexural strength and elastic modulus For a beam in flexure, the maximum outer fibre stress from simple beam theory is: σ fb = M c I where M is the applied moment, c is the distance of the outer fibres (where the tensile force is acting) from the neutral axis, and I is the moment of inertia of the cross section about the neutral axis. It is assumed that the material behaviour is consistent with Hooke s law. For a rectangular test specimen I = bt 3 /2 and c = t/2, where b and t are the width and thickness of the specimen, respectively. With reference to 3-point a configurations, Fig. 6.4, the bending moment can be calculated as M = Replacing the values of M, c and I in eq.(6.) to obtain the flexural bending strength σ fb = P L 4 (6.) (6.2) 3PL 2bt 2 (6.3) From the experimental result, we can also obtain the elastic modulus of the material according to the linearelastic analysis. The deflection of the beam () from the centre as illustrated in Fig. 6.3 can be expressed as δ = PL 3 48 E I where I = wt 3 2. The elastic modulus (E B ) in the above equation can be calculated from the slope of the load-deflection curve (dp/d) in the linear region as follows (6.4) E B = L 3 48 I (dp dδ ) (6.5) E B = m L 3 (6.6) 4 w t 3 where m = (dp/d) is the slope of the tangent to the straight-line portion of the load-deflection beam. 6

7 6.3 The Weibull modulus The strength characterisation data of ceramics reported in terms of flexural bend strength or MOR is relatively inexpensive, straightforward and quick process. But it has severe limitation on the usability of MOR data: the measured strength varies significantly depending on the size of the specimen tested and whether it is loaded in three-point or four-point. Ceramics do not have uniquely defined failure strength. A given batch of ceramic specimens usually does not show a constant measured strength instead they show a range of strengths. The strength of ceramic is determined by a combination of two material parameters the toughness and the crack size. Since fracture toughness is not a variable, the variation in strength comes from a variation in the size of the largest defect (crack), Fig. 6.5, and the microstructure. There are lots of small defects, besides the largest ones, present in the material which are stressed but they do not reach their critical stress for propagation. Hence, it is necessary to use sample sets of ten or more specimens for even the simplest of goals such as determining an average strength for material ranking, material development, or materials specification purposes and a probabilistic approach is needed to interpret test data. Thus, it is also widely recognized that brittle material strengths are statistical in nature. Largest defect Figure 6.4: Flaw distribution in ceramic materials. When analysing the variation in the strength of ceramics, a particular function, due to the Swedish engineer Weibull, has been found to be useful. The simplest form of Weibull approach of characterising the flaw distribution is based on a weakest link model and it is analogous to the breaking of a length of chain. Failure occurs when the weakest link breaks. In a series of chains of a particular length, the weakest link in each length is of different strength and this controls the variation in strength. In ceramics, the links could represent small volumes of material containing a flaw and the weakest link is equivalent to the region with the largest flaw. Considering the two-parameter model, the probability of some length L of a link failing at a stress is P f = P s = exp { ( σ m ) } (6.7) σ 0 Where P f and P s are, respectively, the probability of failure and survival, 0 is a constant called the normalising stress, and m is a number, usually referred to as the Weibull modulus, which reflects the degree of variability in strength the higher the m is, the less variable is the strength. In this Weibull function, the Weibull modulus, m, defines the shape of the failure distribution curve. If m tends to be zero, the failure probability tends to become independent of the applied stress. If m =, the failure probability becomes a simple asymptotic exponential distribution. If m =, the distribution is a step function with P f = 0 when < 0, and P f = when > 0. P f P f m = m = 0 0 7

8 The Weibull modulus, m, also defines the width of the probability distribution, Fig If m is large, the distribution is narrow showing a small spread of failure strength, indicating high reliability of the material. If, on the other hand, m is small, the distribution is wide showing a large variation in the failure strength, indicating unreliability of the material. Poor ceramics have m in the range of 3 0, while good engineering ceramics have m in the range 0 40, and homogeneous metals and alloys have m well above 00. P f P f large m small m 0 0 A substantial number of test samples are required to determine accurate value for the Weibull slope m. Testing of only 0 samples can result in an error as high as ±40% in the m value. Over 80 samples are required to obtain 90% confidence in the m value Determining Weibull parameters from experimental data Taking natural logarithms in both sides of eq.(3.7), we get ln P s = ( σ m ) σ 0 (6.8) Taking natural logarithms again ln ( ln P s ) = m ln σ m ln σ 0 (6.9) ln { ln( P f )} = m ln σ m ln σ 0 (6.0) Thus plotting ln ( ln P s ) or ln ( ln ( P f ) as ordinate against ln as abscissa should give a straight line of the form y = mc + c. Here the gradient of the equation is the Weibull modulus m and the intercept to y-axis is the normalising stress 0 in the form of m ln 0. In the analysis of a number of strength data of a typical material through Weibull statistics, the plotting positions for abscissa are obvious but not the ordinate. The failure probability at a given stress is found by first ranking the failure stresses in order of strength. The failure probability of nth ranked sample from a total of N would be P f =( P s ) =n/(n+). The figure shown below is a Weibull plot of nine fracture strength data of abraded glass rods. The Weibull modulus of the sample is 4.76, indicating very poor reliability of the data. 8

NORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.

NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric

THE DETERMINATION OF FRACTURE STRENGTH FROM ULTIMATE TENSILE AND TRANSVERSE RUPTURE STRESSES

Powder Metallurgy Progress, Vol.3 (003), No 3 119 THE DETERMINATION OF FRACTURE STRENGTH FROM ULTIMATE TENSILE AND TRANSVERSE RUPTURE STRESSES A.S. Wronski, A.Cias Abstract It is well-recognized that the

PURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.

BENDING STRESS The effect of a bending moment applied to a cross-section of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally

4.MECHANICAL PROPERTIES OF MATERIALS

4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stress-strain diagram

Structural Analysis I Chapter 4 - Torsion TORSION

ORSION orsional stress results from the action of torsional or twisting moments acting about the longitudinal axis of a shaft. he effect of the application of a torsional moment, combined with appropriate

Chapter 7. Highlights:

Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true

Mechanics of Materials Primer

Mechanics of Materials rimer Notation: A = area (net = with holes, bearing = in contact, etc...) b = total width of material at a horizontal section d = diameter of a hole D = symbol for diameter E = modulus

MECE 3321 MECHANICS OF SOLIDS CHAPTER 3

MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.

JUT!SI I I I TO BE RETURNED AT THE END OF EXAMINATION. THIS PAPER MUST NOT BE REMOVED FROM THE EXAM CENTRE. SURNAME: FIRST NAME: STUDENT NUMBER:

JUT!SI I I I TO BE RETURNED AT THE END OF EXAMINATION. THIS PAPER MUST NOT BE REMOVED FROM THE EXAM CENTRE. SURNAME: FIRST NAME: STUDENT NUMBER: COURSE: Tutor's name: Tutorial class day & time: SPRING

STRENGTH OF MATERIALS-I. Unit-1. Simple stresses and strains

STRENGTH OF MATERIALS-I Unit-1 Simple stresses and strains 1. What is the Principle of surveying 2. Define Magnetic, True & Arbitrary Meridians. 3. Mention different types of chains 4. Differentiate between

ME 2570 MECHANICS OF MATERIALS

ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation

ME 243. Mechanics of Solids

ME 243 Mechanics of Solids Lecture 2: Stress and Strain Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET E-mail: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil

Mechanical properties 1 Elastic behaviour of materials

MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical

Tensile stress strain curves for different materials. Shows in figure below

Tensile stress strain curves for different materials. Shows in figure below Furthermore, the modulus of elasticity of several materials effected by increasing temperature, as is shown in Figure Asst. Lecturer

Homework No. 1 MAE/CE 459/559 John A. Gilbert, Ph.D. Fall 2004

Homework No. 1 MAE/CE 459/559 John A. Gilbert, Ph.D. 1. A beam is loaded as shown. The dimensions of the cross section appear in the insert. the figure. Draw a complete free body diagram showing an equivalent

Mechanical Properties of Materials

Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of

High Tech High Top Hat Technicians. An Introduction to Solid Mechanics. Is that supposed to bend there?

High Tech High Top Hat Technicians An Introduction to Solid Mechanics Or Is that supposed to bend there? Why don't we fall through the floor? The power of any Spring is in the same proportion with the

Engineering Science OUTCOME 1 - TUTORIAL 4 COLUMNS

Unit 2: Unit code: QCF Level: Credit value: 15 Engineering Science L/601/10 OUTCOME 1 - TUTORIAL COLUMNS 1. Be able to determine the behavioural characteristics of elements of static engineering systems

QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS

QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1- STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State Hooke s law. 3. Define modular ratio,

MATERIALS FOR CIVIL AND CONSTRUCTION ENGINEERS

MATERIALS FOR CIVIL AND CONSTRUCTION ENGINEERS 3 rd Edition Michael S. Mamlouk Arizona State University John P. Zaniewski West Virginia University Solution Manual FOREWORD This solution manual includes

Materials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.

Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie

UNIT I SIMPLE STRESSES AND STRAINS

Subject with Code : SM-1(15A01303) Year & Sem: II-B.Tech & I-Sem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES

[8] Bending and Shear Loading of Beams Page 1 of 28 [8] Bending and Shear Loading of Beams [8.1] Bending of Beams (will not be covered in class) [8.2] Bending Strain and Stress [8.3] Shear in Straight

Flexural properties of polymers

A2 _EN BUDAPEST UNIVERSITY OF TECHNOLOGY AND ECONOMICS FACULTY OF MECHANICAL ENGINEERING DEPARTMENT OF POLYMER ENGINEERING Flexural properties of polymers BENDING TEST OF CHECK THE VALIDITY OF NOTE ON

QUESTION BANK DEPARTMENT: CIVIL SEMESTER: III SUBJECT CODE: CE2201 SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1- STRESS AND STRAIN PART A

DEPARTMENT: CIVIL SUBJECT CODE: CE2201 QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1- STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State

five Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture

ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS

five Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture

ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS

MATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?

MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition

N = N A Pb A Pb. = ln N Q v kt. = kt ln v N

5. Calculate the energy for vacancy formation in silver, given that the equilibrium number of vacancies at 800 C (1073 K) is 3.6 10 3 m 3. The atomic weight and density (at 800 C) for silver are, respectively,

Johns Hopkins University What is Engineering? M. Karweit MATERIALS

Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: MATERIALS A. Composition

Stress-Strain Behavior

Stress-Strain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.

ME Final Exam. PROBLEM NO. 4 Part A (2 points max.) M (x) y. z (neutral axis) beam cross-sec+on. 20 kip ft. 0.2 ft. 10 ft. 0.1 ft.

ME 323 - Final Exam Name December 15, 2015 Instructor (circle) PROEM NO. 4 Part A (2 points max.) Krousgrill 11:30AM-12:20PM Ghosh 2:30-3:20PM Gonzalez 12:30-1:20PM Zhao 4:30-5:20PM M (x) y 20 kip ft 0.2

AERO 214. Lab II. Measurement of elastic moduli using bending of beams and torsion of bars

AERO 214 Lab II. Measurement of elastic moduli using bending of beams and torsion of bars BENDING EXPERIMENT Introduction Flexural properties of materials are of interest to engineers in many different

Name :. Roll No. :... Invigilator s Signature :.. CS/B.TECH (CE-NEW)/SEM-3/CE-301/ SOLID MECHANICS

Name :. Roll No. :..... Invigilator s Signature :.. 2011 SOLID MECHANICS Time Allotted : 3 Hours Full Marks : 70 The figures in the margin indicate full marks. Candidates are required to give their answers

How materials work. Compression Tension Bending Torsion

Materials How materials work Compression Tension Bending Torsion Elemental material atoms: A. Composition a) Nucleus: protons (+), neutrons (0) b) Electrons (-) B. Neutral charge, i.e., # electrons = #

THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH

THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk

ME 354, MECHANICS OF MATERIALS LABORATORY COMPRESSION AND BUCKLING

ME 354, MECHANICS OF MATERIALS LABATY COMPRESSION AND BUCKLING PURPOSE 01 January 2000 / mgj The purpose of this exercise is to study the effects of end conditions, column length, and material properties

MECHANICS OF MATERIALS Sample Problem 4.2

Sample Problem 4. SOLUTON: Based on the cross section geometry, calculate the location of the section centroid and moment of inertia. ya ( + Y Ad ) A A cast-iron machine part is acted upon by a kn-m couple.

FLEXURAL MODELLING OF STRAIN SOFTENING AND STRAIN HARDENING FIBER REINFORCED CONCRETE

Proceedings, Pro. 53, S.A.R.L., Cachan, France, pp.55-6, 7. FLEXURAL MODELLING OF STRAIN SOFTENING AND STRAIN HARDENING FIBER REINFORCED CONCRETE Chote Soranakom and Barzin Mobasher Department of Civil

Lab Exercise #5: Tension and Bending with Strain Gages

Lab Exercise #5: Tension and Bending with Strain Gages Pre-lab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material

CHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS

CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a cross-sectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress

GEOSYNTHETICS ENGINEERING: IN THEORY AND PRACTICE

GEOSYNTHETICS ENGINEERING: IN THEORY AND PRACTICE Prof. J. N. Mandal Department of Civil Engineering, IIT Bombay, Powai, Mumbai 400076, India. Tel.022-25767328 email: cejnm@civil.iitb.ac.in Module-13 LECTURE-

Introduction to Engineering Materials ENGR2000. Dr. Coates

Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed

ENGINEERING SCIENCE H1 OUTCOME 1 - TUTORIAL 4 COLUMNS EDEXCEL HNC/D ENGINEERING SCIENCE LEVEL 4 H1 FORMERLY UNIT 21718P

ENGINEERING SCIENCE H1 OUTCOME 1 - TUTORIAL COLUMNS EDEXCEL HNC/D ENGINEERING SCIENCE LEVEL H1 FORMERLY UNIT 21718P This material is duplicated in the Mechanical Principles module H2 and those studying

12/8/2009. Prof. A.K.M.B. Rashid Department of MME BUET, Dhaka

Prof. A.K.M.B. Rashid Department of MME BUET, Dhaka Introduction and classes of properties Case studies showing selection of the right material for the job Deformation of material under the action of a

PERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR - VALLAM THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK

PERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR - VALLAM - 613 403 - THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Sub : Strength of Materials Year / Sem: II / III Sub Code : MEB 310

: APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4021 COURSE CATEGORY : A PERIODS/ WEEK : 5 PERIODS/ SEMESTER : 75 CREDIT : 5 TIME SCHEDULE

COURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4021 COURSE CATEGORY : A PERIODS/ WEEK : 5 PERIODS/ SEMESTER : 75 CREDIT : 5 TIME SCHEDULE MODULE TOPIC PERIODS 1 Simple stresses

22 Which of the following correctly defines the terms stress, strain and Young modulus? stress strain Young modulus

PhysicsndMathsTutor.com Which of the following correctly defines the terms stress, strain and Young modulus? 97/1/M/J/ stress strain Young modulus () x (area) (extension) x (original length) (stress) /

Bending Load & Calibration Module Objectives After completing this module, students shall be able to: 1) Conduct laboratory work to validate beam bending stress equations. 2) Develop an understanding of

9 MECHANICAL PROPERTIES OF SOLIDS

9 MECHANICAL PROPERTIES OF SOLIDS Deforming force Deforming force is the force which changes the shape or size of a body. Restoring force Restoring force is the internal force developed inside the body

SERVICEABILITY OF BEAMS AND ONE-WAY SLABS

CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach - Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONE-WAY SLABS A. J. Clark School of Engineering Department of Civil

The objective of this experiment is to investigate the behavior of steel specimen under a tensile test and to determine it's properties.

Objective: The objective of this experiment is to investigate the behavior of steel specimen under a tensile test and to determine it's properties. Introduction: Mechanical testing plays an important role

COURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4017 COURSE CATEGORY : A PERIODS/WEEK : 6 PERIODS/ SEMESTER : 108 CREDITS : 5

COURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4017 COURSE CATEGORY : A PERIODS/WEEK : 6 PERIODS/ SEMESTER : 108 CREDITS : 5 TIME SCHEDULE MODULE TOPICS PERIODS 1 Simple stresses

PDDC 1 st Semester Civil Engineering Department Assignments of Mechanics of Solids [ ] Introduction, Fundamentals of Statics

Page1 PDDC 1 st Semester Civil Engineering Department Assignments of Mechanics of Solids [2910601] Introduction, Fundamentals of Statics 1. Differentiate between Scalar and Vector quantity. Write S.I.

CE6306 STRENGTH OF MATERIALS TWO MARK QUESTIONS WITH ANSWERS ACADEMIC YEAR 2014-2015 UNIT - 1 STRESS, STRAIN AND DEFORMATION OF SOLIDS PART- A 1. Define tensile stress and tensile strain. The stress induced

Module III - Macro-mechanics of Lamina. Lecture 23. Macro-Mechanics of Lamina

Module III - Macro-mechanics of Lamina Lecture 23 Macro-Mechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the

Chapter 3. Load and Stress Analysis

Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3

TENSILE TESTS (ASTM D 638, ISO

MODULE 4 The mechanical properties, among all the properties of plastic materials, are often the most important properties because virtually all service conditions and the majority of end-use applications

Sample Questions for the ME328 Machine Design Final Examination Closed notes, closed book, no calculator.

Sample Questions for the ME328 Machine Design Final Examination Closed notes, closed book, no calculator. The following is from the first page of the examination. I recommend you read it before the exam.

2012 MECHANICS OF SOLIDS

R10 SET - 1 II B.Tech II Semester, Regular Examinations, April 2012 MECHANICS OF SOLIDS (Com. to ME, AME, MM) Time: 3 hours Max. Marks: 75 Answer any FIVE Questions All Questions carry Equal Marks ~~~~~~~~~~~~~~~~~~~~~~

Outline. Tensile-Test Specimen and Machine. Stress-Strain Curve. Review of Mechanical Properties. Mechanical Behaviour

Tensile-Test Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress - true strain (flow curve) mechanical properties: - Resilience - Ductility - Toughness - Hardness A standard

Samantha Ramirez, MSE

Samantha Ramirez, MSE Centroids The centroid of an area refers to the point that defines the geometric center for the area. In cases where the area has an axis of symmetry, the centroid will lie along

7.6 Stress in symmetrical elastic beam transmitting both shear force and bending moment

7.6 Stress in symmetrical elastic beam transmitting both shear force and bending moment à It is more difficult to obtain an exact solution to this problem since the presence of the shear force means that

CHAPTER 3 EXPERIMENTAL STUDY

Experimental Study 42 CHAPTER 3 EXPERIMENTAL STUDY 3.1. INTRODUCTION The experimental study that has been carried out in this thesis has two main objectives: 1. Characterise the concrete behaviour in mode

PES Institute of Technology

PES Institute of Technology Bangalore south campus, Bangalore-5460100 Department of Mechanical Engineering Faculty name : Madhu M Date: 29/06/2012 SEM : 3 rd A SEC Subject : MECHANICS OF MATERIALS Subject

UNIT III DEFLECTION OF BEAMS 1. What are the methods for finding out the slope and deflection at a section? The important methods used for finding out the slope and deflection at a section in a loaded

6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and

6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile

COURSE TITLE : THEORY OF STRUCTURES -I COURSE CODE : 3013 COURSE CATEGORY : B PERIODS/WEEK : 6 PERIODS/SEMESTER: 90 CREDITS : 6

COURSE TITLE : THEORY OF STRUCTURES -I COURSE CODE : 0 COURSE CATEGORY : B PERIODS/WEEK : 6 PERIODS/SEMESTER: 90 CREDITS : 6 TIME SCHEDULE Module Topics Period Moment of forces Support reactions Centre

The University of Melbourne Engineering Mechanics

The University of Melbourne 436-291 Engineering Mechanics Tutorial Four Poisson s Ratio and Axial Loading Part A (Introductory) 1. (Problem 9-22 from Hibbeler - Statics and Mechanics of Materials) A short

Measurement of Bone Strength and Stiffness using 3-Point Bending

BME 315 Biomechanics, U. Wisconsin Adapted by R. Lakes from D. Thelen and C. Decker, 09, adapted from Lakes 06 Experimental Details I. Laboratory equipment The load frame that we will use to perform our

Elastic Properties of Solid Materials. Notes based on those by James Irvine at

Elastic Properties of Solid Materials Notes based on those by James Irvine at www.antonine-education.co.uk Key Words Density, Elastic, Plastic, Stress, Strain, Young modulus We study how materials behave

MEASURMENT OF BENDING PROPERTIES OF RHIZOPHORA TROPICAL WOOD. Sarawak, Malaysia. Engineering & Technology, Dhaka, Bangladesh

AJSTD Vol. 26 Issue 2 pp. 73-84 (2010) MEASURMENT OF BENDING PROPERTIES OF RHIZOPHORA TROPICAL WOOD Sinin Hamdan* a, Mahbub Hasan b and Yoann Nohe c a Faculty of Engineering, Universiti Malaysia Sarawak,

Materials and Shape. Part 1: Materials for efficient structure. A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka. Learning Objectives

MME445: Lecture 27 Materials and Shape Part 1: Materials for efficient structure A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Learning Objectives Knowledge & Understanding Understand the

Volume 2 Fatigue Theory Reference Manual

Volume Fatigue Theory Reference Manual Contents 1 Introduction to fatigue 1.1 Introduction... 1-1 1. Description of the applied loading... 1-1.3 Endurance curves... 1-3 1.4 Generalising fatigue data...

X has a higher value of the Young modulus. Y has a lower maximum tensile stress than X

Bulk Properties of Solids Old Exam Questions Q1. The diagram shows how the stress varies with strain for metal specimens X and Y which are different. Both specimens were stretched until they broke. Which

MECE 3321: Mechanics of Solids Chapter 6

MECE 3321: Mechanics of Solids Chapter 6 Samantha Ramirez Beams Beams are long straight members that carry loads perpendicular to their longitudinal axis Beams are classified by the way they are supported

Mechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering

Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected

A concrete cylinder having a a diameter of of in. mm and elasticity. Stress and Strain: Stress and Strain: 0.

2011 earson Education, Inc., Upper Saddle River, NJ. ll rights reserved. This material is protected under all copyright laws as they currently 8 1. 3 1. concrete cylinder having a a diameter of of 6.00

Influence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes

October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:

Essentially, all models are wrong, but some are useful George E.P. Box, (Box and Draper, 1987) 5 ADVANCED FRACTURE MODELS In the previous chapter it was shown that the MOR parameter cannot be relied upon

FCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering

FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001-015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress

CHAPTER 6: ULTIMATE LIMIT STATE

CHAPTER 6: ULTIMATE LIMIT STATE 6.1 GENERAL It shall be in accordance with JSCE Standard Specification (Design), 6.1. The collapse mechanism in statically indeterminate structures shall not be considered.

Russell C. Hibbeler. Chapter 1: Stress

Russell C. Hibbeler Chapter 1: Stress Introduction Mechanics of materials is a study of the relationship between the external loads on a body and the intensity of the internal loads within the body. This

In Situ Ultrasonic NDT of Fracture and Fatigue in Composites

ECNDT 26 - Mo.2.6.5 In Situ Ultrasonic NDT of Fracture and Fatigue in Composites I. SOLODOV, K. PFLEIDERER, and G. BUSSE Institute for Polymer Testing and Polymer Science (IKP), Non-destructive Testing

THEME IS FIRST OCCURANCE OF YIELDING THE LIMIT?

CIE309 : PLASTICITY THEME IS FIRST OCCURANCE OF YIELDING THE LIMIT? M M - N N + + σ = σ = + f f BENDING EXTENSION Ir J.W. Welleman page nr 0 kn Normal conditions during the life time WHAT HAPPENS DUE TO

NAME: Given Formulae: Law of Cosines: Law of Sines:

NME: Given Formulae: Law of Cosines: EXM 3 PST PROBLEMS (LESSONS 21 TO 28) 100 points Thursday, November 16, 2017, 7pm to 9:30, Room 200 You are allowed to use a calculator and drawing equipment, only.

Tuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE

1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & Free-Body Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for

Lecture 15 Strain and stress in beams

Spring, 2019 ME 323 Mechanics of Materials Lecture 15 Strain and stress in beams Reading assignment: 6.1 6.2 News: Instructor: Prof. Marcial Gonzalez Last modified: 1/6/19 9:42:38 PM Beam theory (@ ME

TORSION TEST. Figure 1 Schematic view of torsion test

TORSION TEST 1. THE PURPOSE OF THE TEST The torsion test is performed for determining the properties of materials like shear modulus (G) and shear yield stress ( A ). 2. IDENTIFICATIONS: Shear modulus:

KINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK. Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV

KINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV UNIT I STRESS, STRAIN DEFORMATION OF SOLIDS PART A (2 MARKS)

Earthquake-resistant design of indeterminate reinforced-concrete slender column elements

Engineering Structures 29 (2007) 163 175 www.elsevier.com/locate/engstruct Earthquake-resistant design of indeterminate reinforced-concrete slender column elements Gerasimos M. Kotsovos a, Christos Zeris

(1) Brass, an alloy of copper and zinc, consists of 70% by volume of copper and 30% by volume of zinc.

PhysicsAndMathsTutor.com 1 Q1. (a) Define the density of a material....... (1) (b) Brass, an alloy of copper and zinc, consists of 70% by volume of copper and 30% by volume of zinc. density of copper =

CHAPTER 4: BENDING OF BEAMS

(74) CHAPTER 4: BENDING OF BEAMS This chapter will be devoted to the analysis of prismatic members subjected to equal and opposite couples M and M' acting in the same longitudinal plane. Such members are

CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES

CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric

MECHANICS LAB AM 317 EXP 3 BENDING STRESS IN A BEAM

MECHANICS LAB AM 37 EXP 3 BENDING STRESS IN A BEAM I. OBJECTIVES I. To compare the experimentally determined stresses in a beam with those predicted from the simple beam theory (a.k.a. Euler-Bernoull beam

DEPARTMENT OF CIVIL ENGINEERING

KINGS COLLEGE OF ENGINEERING DEPARTMENT OF CIVIL ENGINEERING SUBJECT: CE 2252 STRENGTH OF MATERIALS UNIT: I ENERGY METHODS 1. Define: Strain Energy When an elastic body is under the action of external